SIL ET AL . VOL. 8 ’ NO. 8 ’ 7755–7762 ’ 2014
July 29, 2014
C 2014 American Chemical Society
Seeing Is Believing: Hot ElectronBased Gold Nanoplasmonic
OpticalHydrogen SensorDevika Sil,† Kyle D. Gilroy,‡ Aurelia Niaux,†
Abdelaziz Boulesbaa,† Svetlana Neretina,‡ and Eric Borguet†,*
†Department of Chemistry, Temple University, Philadelphia,
Pennsylvania 19122, United States and ‡College of Engineering,
Temple University, Philadelphia,Pennsylvania 19122, United
The interaction of metal nanoparticles(NPs) with photons whose
energy isresonant with the surface plasmon
leads to the generation of plasma oscilla-tions which can decay
into hot electrons.1�3
This strong interaction offers the opportu-nity to couple light
to drive chemical reac-tions and provides a means to
generatevaluable product with relatively low energyinput.2 The
probability of generating ther-malized, or “hot”, electrons is
increasedwhen the metal nanoparticles are muchsmaller than the
wavelength of the incidentradiation.2
Recent studies have focused on the trans-fer of hot electrons
from excited metalsurfaces to nearby molecular orbitals.2,3
Mukherjee et al. provided the first experi-mental evidence for
the room-temperaturephotocatalytic dissociation of H2 on 5�30
nmgold nanoparticles using visible light.2,3 Theirresults
demonstrated that a fraction of thehot electrons generated by the
resonantlyexcited gold nanoparticles allowed for elec-tron transfer
into the 1σu* antibonding orbi-tal of a physisorbed H2 molecule,
dissociation.2,3 The requirements for thisprocess are that (i)
the Au NPs are excitedresonantly, (ii) the Feshbach energy
overlapsthe hot electron distribution,4 (iii) the hotelectrons have
energy greater than 1.8 eV,(iv) the weight fraction of Au in TiO2,
or SiO2,is between 0.5% and 3%,2,3 and (v) the nano-particles are
sufficiently small (
SIL ET AL . VOL. 8 ’ NO. 8 ’ 7755–7762 ’ 2014
scheme using the localized surface plasmon resonance(LSPR) was
reported.17�23 The LSPR is a sensitive probeof changes in the local
environment, such as perturba-tions in the dielectric properties of
the medium. Thecollective oscillations of free electrons are driven
bythe interaction of plasmonic metallic nanoparticles(typically Au,
Ag, or Cu) with visible light.24 Indirectnanoplasmonic sensing
schemes employ an enhancedelectric field to sense changes in the
dielectric envi-ronment triggered by a secondary activematerial,
suchas Pd. When placed in the near-field of resonantlyexcited Au
nanoparticles, an external analyte molecule(e.g., H2) changes the
dielectric properties of Pd, whichin turn shifts the LSPR of the Au
nanoparticles.17�23 Pdwas chosen due to its well-established
ability to dis-sociate and absorb hydrogen and undergo a
reversiblelattice expansion.25,26 As shown by Liu et al., as the
PdNP approaches the near-field of a resonantly excitedAu
nanotriangle, the spectral position and scatteringintensity of the
Au system shift upon hydrogen ex-posure due to the formation of Pd
hydride, which hasdifferent dielectric properties compared to Pd.22
Lan-ghammer et al. used substrate-based Au nanodisksseparated from
Pd nanoparticles by a thin dielectricspacer layer to study
hydriding and dehydridingkinetics of 1.8�5.4 nm Pd nanoparticles.23
However,Liu et al. and Langhammer et al. did not report anyhydrogen
sensingwith the Au nanostructures alone.22,23
The discovery of the hot electron induced photocatalyticactivity
of Au nanoparticles by Mukherjee et al.2,3 showsthat the Au LSPR
could drive the dissociation of H2without the need for an adjacent
active material suchas Pd. However, any change in the optical
response ofthe Au nanoparticles due to hot electron induced
dis-sociation of hydrogen has yet to be reported.The interaction of
Au with hydrogen, especially the
formation of Au�H bonds, is far from being under-stood due to
the inert nature of bulk Au. However,there are studies, both
theoretical and experimental,that discuss the adsorption of
hydrogen onto Au27�30
and the formation of AuHx.30�37 Bus et al. reported that
small gold nanoparticles (∼1.4 nm) supported on alu-mina
dissociatively adsorb hydrogen.30 This is accom-panied by a change
in electronic properties, as it wasshownbyX-ray absorptionnear-edge
spectroscopy thatthe L3,2 edges of Au/Al2O3 recorded in hydrogen
under-go a shift of several electronvolts.30 Previous reports
alsomentioned that the formation of surface-based AuH2
and AuH4� is stabilized by relativistic effects38 and is
likely to occur in electron-rich systems such as providedby
laser ablation and plasmas.34 The catalytic activitywas associated
with atomic sites of lower coordination(i.e., at the edges and
corners).In this work, we optically detect the dissociation of
H2 on Au nanoparticles. The novelty stems from
theroom-temperature optical detection of hydrogenusing (i)
thermally self-assembled substrate-based
gold nanohemispheres (Au NHs) and (ii) surfactant-free
structures (allowing for close contact between thenanostructures
and the analyte). It is important to notethat the observation of
hot electron generation forspherical, larger nanostructures (>20
nm) was pre-viously reported to be negligible2,4,39 and that
thedissociation of H2 was negligible.
2,4,40,41 On the con-trary, in the present study, a∼1�2% change
in opticaltransmission was achieved at room temperature usingAu NHs
between 10 and 50 nm in diameter upon inco-herent excitation. To
substantiate the claim of AuHxformation, discrete dipole
approximation (DDA) simu-lationswere carried out using dielectric
constants of Auhydride previously measured by Giangregorio et
Characterization of Films. Tapping mode atomicforce microscope
(AFM) images of the Au NHs film(Figure 1a) showed a broad
distribution of closelyspaced hemispherical particles between 10
and50 nm. A histogram is shown in Figure 1b, where theaverage size
was measured to be∼28( 8 nm. The UV/vis extinction spectrum (Figure
1c) showed the plas-mon band of Au NHs as a wide
inhomogeneouslybroadened feature at ∼570 nm. The peak
positionappeared to be red-shifted by about 50 nm from
thepreviously reported position of plasmon band forspherical Au
NPs.42 This shift in spectral position ofthe plasmon band could be
attributed to two effects:(a) nanoparticle shape induced effects
and (b) nano-particle size related changes in surface plasmon
reso-nance. The geometry-induced shift was observedpreviously for
other metals43 and was attributed tothe effective dipole being
closer to the substrate. It wasfound that hemispheres have a
stronger interactionwith the substrate as compared to spheres.43,44
Nano-particle dimension induced changes in the surfaceplasmon
resonance arise due to increased electromag-netic retardation in
larger nanoparticles.45,46 In thepresent case, the red shift could
be a cumulative resultof the two aforementioned phenomena.
Plasmonic Sensing Results. The broadband incoherentexcitation
was selected to cover wavelengths between500�600 nm and the real
time response of the Au film(Figure 2a�c) in H2 wasmonitored. An
average increaseof∼1.8% in the transmitted intensity through an Au
NHfilm, supported on a glass slide, was observed within0.3�1 s of
turning onH2. TheAuNH filmwas exposed to10% H2 in N2 for 10�20 s,
during which time thetransmitted intensity stayed constant. Upon
turningoff the H2 flow, the transmitted intensity recovered tothe
initial value. Thus, from the real-time monitoring ofthe response
of Au NHs to H2 (Figure 2), it becameevident that these
nanostructures act as rapid andreusable optical H2 sensors upon
resonant excitationat the SPR. Details regarding the experimental
setup areprovided in the Supporting Information (SI, Figure
SIL ET AL . VOL. 8 ’ NO. 8 ’ 7755–7762 ’ 2014
Hydriding and Dehydriding of Au NHs with UV/Vis Spectros-copy.
The surface plasmon resonance of Au NHs filmswas tracked with and
without hydrogen exposure byrecording transmission spectra with a
UV/vis spectro-meter. In the absence of hydrogen the signal
stayedstable at a transmittance of ∼46%. Upon introducinghydrogen,
a ∼1% increase in transmittance was
observed (Figure 3). After stopping H2 and waiting,the
transmittance signal recovered to the initial value.The presence of
hydrogen induced a blue shift of∼3 nm.
Wavelength Dependence. Combinations of filters wereplaced in the
beam path to vary the incident excita-tion wavelength range (See
Figure S4 in SI for details)in order to study how it affected the
magnitudeof the optical response of the Au NH films to hydro-gen.
The experiments were carried out at 293 Kand under similar
illumination intensities coveringphoton wavelengths from 400�800
nm. The changein transmission was greatest for wavelengthswithin 30
nm of the LSPR (λex = 550 and 580 nm)(Figure 4).
Figure 2. Real-time monitoring of changes in
transmittedintensity for multiple cycles of H2. Each point plotted
isthe percentage change in transmitted intensity between500 and 600
nm as a function of time. Each time incrementwas 0.3 s apart. Rapid
response after (a) seven cycles ofhydrogen, (b) 11 cycles of
hydrogen, and (c) one cycle ofhydrogen close up to show both the ON
Figure 3. Tracking the surface plasmon resonance of AuNHs in H2
with a UV/vis spectrometer. Red spectrum iswithout anyH2; blue
spectrumdisplays the optical responseduring hydrogen; and green is
after the hydrogen isstopped. The presence of hydrogen causes a
reversible1% change in transmittance.
Figure 1. Morphological and optical characterization of a
thermally assembledAu film.Morphological characterization
usingtapping mode AFM on (a) dewetted Au NHs and (b) histogram
showing particle size distribution of Au NHs, with an averagesize
of 28 ( 8 nm. (c) UV/vis extinction spectra of the Au NH film and
of a blank slide.
SIL ET AL . VOL. 8 ’ NO. 8 ’ 7755–7762 ’ 2014
The question as to why Au nanoparticle surfaces arereactive to
hydrogen when their LSPR is excited wasrecently answered by
Mukherjee et al.2 They provideda mechanism of hot electron induced
dissociation ofhydrogen on Au nanoparticles and showed the
forma-tion of HD from a constant flow of H2 and D2 onsupported Au
catalysts. On the basis of themechanismput forward by Mukherjee et
al.2 and the agreement ofexperimental observations with theoretical
calcula-tions, we believe the optical change could be happen-ing
through the following steps:
(a) Optical excitation is resonant with the LSPR ofAu
(b) Coherent plasmons decay into hot electrons(c) A fraction of
the hot electrons undergo electron
transfer into the H2 1σu* antibonding orbital,which leads to H2
(d) Dissociated hydrogen atoms adsorb and diffuseinto Au NHs to
form a metastable Au hydride
AuþH2 f Au� H (1)
Au� HþH f AuþH2v (2)(e) Metastable Au hydride has a different
constant than Au. The change in dielectricconstants modifies the
LSPR position of theparticles and the optical transmission of
(f) In the absence of a steady flux of H2, there is anet
diffusion of H atoms out from nanoparticlethin film leading to
recovery of the initial opticalproperties.
The formation of the metastable Au hydride inducesa spectral
shift and change in transmitted intensity,which are explained as
Spectral Shift in Au LSPR in the Presence of Hydrogen Dueto
Electron Transfer. The surface plasmon resonance
condition is approximately fulfilled when
ε1 ¼ �2εm (3)where ε1 is the real part of the dielectric
constant of themetal and εm is the dielectric constant of the
embed-ding medium of the nanoparticles.34 The Drude modelpredicts
that the dielectric constants of metals dependon the plasmon
frequency as follows:
εD(ω) ¼ 1 � ωp2
ω2 þ iγω (4)
ωp2 ¼ ne
ωp is the plasmon frequency, γ is the damping con-stant, n is
the electron density, e is the electron charge,εo is the
permittivity in a vacuum, and meff is theeffective mass of the
electron. Since the plasmonfrequency varies as the square root of
electron density,any change in the number of electrons (i.e.,
addition orremoval of electrons from the metallic core) will
shiftthe position of the surface plasmon resonance. There-fore, a
blue shift in the position of the surface plasmonupon hydrogenation
implies an increase in electrondensity, hence a more negative
dielectric constant,which is consistent with the slight spectral
shift of3 nm observed in Au LSPR in H2 (Figure 3). Our
opticalsimulations also show that, in order to observe a 1%increase
in transmission and a 3 nm blue shift in Au NHLSPR due to
hydrogenation, the real and imaginaryparts of the dielectric
constant of Au need to change byroughly 2% (SI, Figure S3).
Therefore, the probability ofthe presence of ametastable Au
hydridewith dielectricconstants different than pure Au due to
adsorption ofhydrogen cannot be ruled out.
Au hydride was observed by Strobiriski et al. andBus et al.36,47
Thus, based on the change in transmis-sion and the blue shift of Au
(Figures 2, 3) in hydrogenand agreement with optical calculations
(SI, Figure S3),we speculate that the change in optical
transmissionresults from the formation of a metastable gold
hy-dride due to the adsorption of hydrogen atoms.
Wavelength Dependence of Magnitude of Change in
OpticalTransmission. The dependence of the magnitude of theoptical
change on the wavelength of excitation is also amajor indicator of
a plasmon-driven chemical process.2,3,6
Therefore, the excitationwavelengthswere tuned in orderto excite
at various photon energies (Figure 4) close(within 30 nm) and far
(70�100 nm) from the LSPRpeak of Au NH. Our results show that when
the centralwavelength of excitation was within 30 nm of theLSPR,
the optical transmission increased by ∼1�2%.Upon excitation with
wavelengths further away(70�100 nm) from the peak of the LSPR, the
magni-tude of the optical change in transmission is less,typically
a factor of 4 lower. Outside this window of
Figure 4. Effect of excitation wavelength on themagnitudeof
change in the transmission of Au films in hydrogen.Excitations
within 50 nm of the LSPR of Au NHs (570 nm)demonstrate larger
changes in transmittance. The LSPR ofthe Au NH film is indicated by
the yellow dotted line.
SIL ET AL . VOL. 8 ’ NO. 8 ’ 7755–7762 ’ 2014
near-resonant photon energies, smaller changes areobserved due
to a variety of reasons including (i) fewerhot electrons are
generated and (ii) the (e��H2) inter-action probability is low.
Mukherjee et al. observedsimilar results for plasmonic HD
generation and men-tioned that “since the absorption cross section
corre-sponds directly to the hot electron production rate,this
provides direct evidence for plasmon-inducedhot-electron-driven H2
2 Christopheret al. also reported similarity in the wavelength
depen-dence of ethylene epoxidation rates due to dissocia-tion of
oxygen on Ag nanocubes and the LSPRspectrum of the silver nanocube
catalysts used.6 Thiscorrelation between the wavelength dependence
ofplasmon-induced reactions and the LSPR spectrum ofmetallic
nanocatalysts at constant illumination inten-sity provides evidence
that the resonant LSPR excita-tion is responsible for the
Confinement of the Electric Field. Finite difference timedomain
(FDTD) simulations were performed to identifythe origin of the
photocatalytic response of large(>20 nm) Au NHs. We compared the
nature of theelectric field enhancement of substrate-based
Auspheres and Au NHs, both 30 nm in diameter, usingFDTD. The
simulation (Figure 5) demonstrated that,upon resonant excitation,
the Au NHs generatestrong fields near the surface of the substrate.
The AuNHs exhibit maximum enhancement at ∼550 nm
(Figure 5e), which is the calculated surface plasmonresonance of
a 30 nm Au hemisphere positioned onSiO2. The UV/vis spectrum of Au
NHs showed a plas-mon resonance at 570 nm. This red shift could
beattributed to the presence of larger particles arisingfrom the
polydispersity in nanoparticle size distribu-tion. The spherical Au
nanoparticles exhibited themaximum enhancement of 1.3 times at 530
nm(Figure 5b) at the LSPR wavelength. On the other hand,the 30 nm
Au NHs showed 2.3 times enhancement atits LSPR (570 nm) (Figure
5e). It was evident that off-resonance, e.g., 500 and 700 nm
(Figure 5a, c, d, f), theelectric field was weaker than at the LSPR
for bothgeometries. The AuNHs exhibited approximately twiceas much
confinement of the electric field as thespheres of similar
dimensions. The confinement inthe hemisphere was localized at the
interface withthe substrate, which we suggest is the hot spot for
theplasmon-induced reactions reported here.
Absence of Surfactants or Ligands. Another factor thatpossibly
enhances the efficiency of the hot electroninduced dissociation is
the absence of any surfactantsor ligands on the thermally dewetted
Au NHs. Therate of hot electron cooling determines the lifetimeof
the energetic electrons and is known to dependon the electronic
heat capacity and the magnitude ofelectron�phonon coupling. Aruda
et al. described howthe hot electron cooling process is affected by
Figure 5. FDTD-simulated electric fields at different
wavelengths for an SiO2 substrate with a single Au sphere on
(a,b,c) or asingle Au hemisphere (d,e,f). The near field
enhancements for the Au sphere on the SiO2 substrate were computed
at (a)500 nm (b) 530 nm-LSPR (c) 700 nm. The nearfield enhancements
for the Auhemisphere on SiO2were calculated at (d) 500 nm(e) 550
nm-LSPR (f) 700 nm. Schematics on the left show the geometry used
for the simulation aswell as the orientation of theincident
k-vector (normal to the surface) and the E-field (y component). At
530 nm, a 1.3� enhancement was observed for the30 nmAu sphere. At
550 nm, a 2.3� enhancement was observed at the edge of the
hemisphere. Au NHs showed about 1.75�more resonant E-field
enhancement in comparison to the sphere at the LSPR.
SIL ET AL . VOL. 8 ’ NO. 8 ’ 7755–7762 ’ 2014
presence of an organic adlayer on a nanoparticle.1,48
The electronic states of metals are known to mix withthat of
organic adsorbates,making the density of statesof passivated metal
nanoparticles considerably differ-ent from that of the bulk. Such
intermixing of electronicstates can significantly alter the
electronic heat capa-city. A summary of prior investigations on
this effectcan be found in Aruda et al.1 The magnitude
ofelectron�phonon coupling also varies from materialto material and
is also dependent on the density ofelectronic states of the system
near the Fermi level andthe distribution of vibrational modes.
Therefore, anyadsorption of ligands or surfactants or changes in
latticestructurewill influence thehotelectroncooling rate.1
Sinceour system is relatively simple, devoid of any
protectivelayer, the hot electron lifetime is most likely
unaffected,which in turn induces efficient hydrogen dissociation
onAu. This makes the resonantly excited Au surface moreresponsive
Probable Presence of Defects. Another factor that
couldcontribute to the enhanced activity of Au NHs is thepresence
of twin boundaries or stacking faults, whichare usually present in
Au nanoparticles of similardimensions.49 The presence of such
defects are known
to enhance catalytic activity by lowering the dissocia-tion
barrier.49�51 Thus, the enhanced reactivity of theAu NHs could be
due to the combined effects of thegeometry, the absence of
surfactants, and the pre-sence of defects.
In this work, we demonstrated that thermally as-sembled Au NHs
provide a platform for the plasmonicdetection of H2. It was also
concluded that plasmonicdetection of H2 was primarily contingent
upon theresonant excitation of the localized surface
plasmons.Investigations into wavelength dependence showedthat
resonantly excited Au NHs show the greatestincrease in
hydrogen-induced optical transmission,confirming the electronic
origin of the response. Nu-merical simulations support the
assertion that theformation of a metastable AuHx can change the
di-electric properties of the films enough to be detectedoptically.
To conclude, we believe that the simplicity ofthis optical
detection system, coupled with the abilityto observe small changes
occurring on subsecond timescales under equilibrium conditions,
will open up othersensing possibilities.
MATERIALS AND METHODSPreparation of Au NH Films. Substrate-based
were producedusing thermal dewetting.52 This process involvestwo
steps: (i) sputter deposition (Gatan high resolution ion beamcoater
model 681) of a 10 nm Au thin film onto sodalime silicamicroscope
glass slides (the resultant film is blue in color) and then(ii)
heating from room temperature to 500 �C in 15 min
(LindbergBlueMtube furnace, TF55035A-1) followedbycoolingback to
roomtemperature. All samples were heated in a constant flow of
ultrahigh purity argon at 65 sccm. The assembled Au
nanostructureshave a hemispherical morphology and are pink in
Characterization. The morphology of Au NHs was assessedusing AFM
tapping mode images recorded using an Agilent5500 scanning probe
microscope with Si3N4 tips (Vista Probes)and processed using
Gwyddion software.53 The histograms werecomputed using ImageJ (NIH)
on a minimum of 100 randomlyselected nanoparticles. UV/vis
spectroscopy was carried out usinga JASCO V570 spectrophotometer
for the characterization ofoptical extinction. An Evolution 201
UV/vis spectrometer was usedto study spectral behavior of hydriding
and dehydriding of Aunanoparticles (wavelength range 190�700 nm,
bandwidth 1 nm,integration time 0.1 s, data interval 1 nm, scan
speed 600 nm/min).
Simulation of Optical Properties. Simulations were done
usingDDSCAT 7.2.0 to explain the changes in dielectric constants
ofAu upon hydrogenation.54 DDSCAT is a software package thatuses
numerical methods to solve for an object's optical re-sponse (i.e.,
absorption and scattering). It uses a 3D array ofpolarizable points
to represent the simulated continuum. Thekey parameters are (i) the
optical properties of the material andsurroundings and (ii) the
object's geometry. In this case, di-electric coefficients for Au
were taken from Palik.55 The di-electric constants of AuHx were
previously measured valuesreported by Giangregorio et al.34
The hemispherical file was modeled using LAMMPSMolecular
Dynamics Simulator56 and was designed so thatthe incident photon
will penetrate directly through the topof the structure, as would
be done in the experiment. The E-fieldis oscillating parallel to
the substrate, while the k-vector isperpendicular. The structure
was modeled using N > 50k
dipoles. The effective radius of the structure is 40 nm, which
isequivalent to a hemisphere with a 44.7 nm radius, yielding anLSPR
centered at 561 nm.
Electromagnetic Simulation. Three-dimensional finite differ-ence
time domain methods (Lumerical FDTD Solutions) wereused to
calculate the near-field properties of resonantly excitedAu spheres
and hemispheres. Nanoparticles with 30 nm di-ameter were chosen to
closely match experimental conditions.A mesh size of 0.8 nm was
chosen for all cases. The simulatedexcitation source took the form
of a polarized Mie source(500�700 nm) penetrating the structure
with a k-vector normalto the substrate surface.
Experimental Setup. The details about the optical sensingsetup
can be found in the SI (Figure S1).
Conflict of Interest: The authors declare no competingfinancial
Supporting Information Available: Figure S1 describes
theexperimental setup, Figure S2 shows the plots of real
andimaginary parts of the refractive index of Au and AuHx, FigureS3
is simulation of extinction spectra of Au and Au hydride, andFigure
S4 shows the spectrum of the filters used for thewavelength
dependence study. This material is available freeof charge via the
Internet at http://pubs.acs.org.
Acknowledgment. Support of this research by the ArmyResearch
Laboratory through contract W911NF-10-2-009 isgratefully
acknowledged. K.D.G. acknowledges support provideby a Temple
University Graduate Fellowship. S.N. acknowledgesthe NSF
(DMR-1053416) CAREER Award. The authors wouldlike to acknowledge
the help of undergraduate students,S. J. Sylla and C. Murphy for
helping with data acquisition.
REFERENCES AND NOTES1. Aruda, K. O.; Tagliazucchi, M.; Sweeney,
C.M.; Hannah, D. C.;
Weiss, E. A. The Role of Interfacial Charge
Transfer-TypeInteractions in the Decay of Plasmon Excitations in
MetalNanoparticles.Phys. Chem. Chem. Phys.2013, 15, 7441–7449.
SIL ET AL . VOL. 8 ’ NO. 8 ’ 7755–7762 ’ 2014
2. Mukherjee, S.; Libisch, F.; Large, N.; Neumann, O.; Brown,L.
V.; Cheng, J.; Lassiter, J. B.; Carter, E. A.; Nordlander,
P.;Halas, N. J. Hot Electrons Do the Impossible: Plasmon-Induced
Dissociation of H2 on Au. Nano Lett. 2012, 13,240–247.
3. Mukherjee, S.; Zhou, L.; Goodman, A. M.; Large, N.;
Ayala-Orozco, C.; Zhang, Y.; Nordlander, P.; Halas, N. J.
Hot-Electron-InducedDissociation of H2 onGoldNanoparticlesSupported
on SiO2. J. Am. Chem. Soc. 2014, 136, 64–67.
4. Murdoch, M.; Waterhouse, G. I. N.; Nadeem, M. A.; Metson,J.
B.; Keane, M. A.; Howe, R. F.; Llorca, J.; Idriss, H. The Effectof
Gold Loading and Particle Size on Photocatalytic Hydro-gen
Production from Ethanol over Au/TiO2 Nanoparticles.Nat. Chem. 2011,
5. Bastus, N. G.; Casals, E.; Ojea, I.; Varon, M.; Puntes, V.
TheDelivery of Nanoparticles. In The Reactivity of
ColloidalInorganic Nanoparticles; Hashim, D. A. A., Ed.; InTech,
6. Christopher, P.; Xin, H.; Linic, S.
Visible-Light-EnhancedCatalytic Oxidation Reactions on Plasmonic
Silver Nano-structures. Nat. Chem. 2011, 3, 467–472.
7. Mubeen, S.; Lee, J.; Singh, N.; Krämer, S.; Stucky, G.
D.;Moskovits, M. An Autonomous Photosynthetic Device inWhich All
Charge Carriers Derive from Surface Plasmons.Nat. Nanotechnol.
2013, 8, 247–251.
8. Thomann, I.; Pinaud, B. A.; Chen, Z.; Clemens, B.M.;
Jaramillo,T. F.; Brongersma, M. L. Plasmon Enhanced
Solar-to-FuelEnergy Conversion. Nano Lett. 2011, 11, 3440–3446.
9. Schwede, J. W.; Bargatin, I.; Riley, D. C.; Hardin, B.
E.;Rosenthal, S. J.; Sun, Y.; Schmitt, F.; Pianetta, P.; Howe,R.
T.; Shen, Z.-X. Photon-Enhanced Thermionic Emissionfor Solar
Concentrator Systems.Nat.Mater.2010, 9, 762–767.
10. Renzas, J. R.; Somorjai, G. A. Rh Thin-Film Nanocatalysts
asChemical Sensors�the Hot Electron Effect. J. Phys. Chem. C2010,
11. Joy, N. A.; Janiszewski, B. K.; Novak, S.; Johnson, T. W.;
Oh,S.-H.; Raghunathan, A.; Hartley, J. G.; Carpenter,M. A.
ThermalStability of Gold Nanorods for High-Temperature
PlasmonicSensing. J. Phys.Chem. C 2013, 117, 11718–11724.
12. Maillard, M.; Huang, P.; Brus, L. Silver Nanodisk Growth
bySurface Plasmon Enhanced Photoreduction of Adsorbed[Agþ]. Nano
Lett. 2003, 3, 1611–1615.
13. Hou, W.; Hung, W. H.; Pavaskar, P.; Goeppert, A.; Aykol,
M.;Cronin, S. B. Photocatalytic Conversion of Co2 to Hydro-carbon
Fuels viaPlasmon-Enhanced Absorption andMetallic Interband
Transitions. ACS Catal. 2011, 1, 929–936.
14. Conklin, D.; Nanayakkara, S.; Park, T.-H.; Lagadec, M.
F.;Stecher, J. T.; Chen, X.; Therien, M. J.; Bonnell, D.
A.Exploiting Plasmon-Induced Hot Electrons in MolecularElectronic
Devices. ACS Nano 2013, 7, 4479–4486.
15. Wu, F.; Tian, L.; Kanjolia, R.; Singamaneni, S.; Banerjee,
P.PlasmonicMetal-to-Semiconductor Switching in AuNano-rod-ZnO
Nanocomposite Films. ACS Appl. Mater. Interfaces2013, 5,
16. Li, C.; Zhang, Y.; Cole, M. T.; Shivareddy, S. G.; Barnard,
J. S.;Lei, W.; Wang, B.; Pribat, D.; Amaratunga, G. A. J.; Milne,
W. I.Hot Electron Field Emission via Individually
Transistor-Ballasted Carbon Nanotube Arrays. ACS Nano 2012,
17. Pavan Kumar, G. V.; Raghuwanshi, M. Palladium AdjoinedGold
Split-Ring Resonators: A Prospective NanoplasmonicHydrogen Sensor.
Opt. Commun. 2013, 300, 65–68.
18. Dasgupta, A.; Kumar, G. V. Palladium Bridged Gold
Nano-cylinder Dimer: Plasmonic Properties and Hydrogen
Sen-sitivity. Appl. Opt. 2012, 51, 1688–1693.
19. Tang, M. L.; Liu, N.; Dionne, J. A.; Alivisatos, A. P.
Observa-tions of Shape-Dependent Hydrogen Uptake Trajectoriesfrom
Single Nanocrystals. J. Am. Chem. Soc. 2011, 133,13220–13223.
20. Shegai, T.; Johansson, P.; Langhammer, C.; Käll,
M.Directional Scattering and Hydrogen Sensing by BimetallicPd-Au
Nanoantennas. Nano Lett. 2012, 12, 2464–2469.
21. Tittl, A.; Kremers, C.; Dorfmuller, J.; Chigrin, D. N.;
Giessen,H. Spectral Shifts in Optical Nanoantenna-EnhancedHydrogen
Sensors. Opt. Mater. Express 2012, 2, 111–118.
22. Liu, N.; Tang, M. L.; Hentschel, M.; Giessen, H.;
Alivisatos,A. P. Nanoantenna-Enhanced Gas Sensing in a
SingleTailored Nanofocus. Nat. Mater. 2011, 10, 631–636.
23. Langhammer, C.; Zhdanov, V. P.; Zori�c, I.; Kasemo, B.
Size-Dependent Kinetics of Hydriding and Dehydriding of
PdNanoparticles. Phys. Rev. Lett. 2010, 104, 135502.
24. Kelly, K. L.; Coronado, E.; Zhao, L. L.; Schatz, G. C.
TheOptical Properties of Metal Nanoparticles: The Influence ofSize,
Shape, and Dielectric Environment. J. Phys. Chem. B2003, 107,
25. Flanagan, T. B.; Oates, W. A. The Palladium-HydrogenSystem.
Annu. Rev. Mater. Sci. 1991, 21, 269–304.
26. Lewis, F. A. The Palladium Hydrogen System; AcademicPress:
London, 1967; Vol. 124.
27. Wang, Y.; Gong, X. G. First-Principles Study of
Interactionof Cluster Au32 with CO, H2, and O2. J. Chem. Phys.
28. Csonka, S.; Halbritter, A.; Mihaly, G.; Jurdik, E.;
Shklyarevskii, O.; Speller, S.; Van Kempen, H. Fractional
Conductancein Hydrogen-Embedded Gold Nanowires. Phys. Rev.
Lett.2003, 90, 116803.
29. Jelínek, P.; Pérez, R.; Ortega, J.; Flores, F. Hydrogen
Dis-sociation over Au Nanowires and the Fractional Conduc-tance
Quantum. Phys. Rev. Lett. 2006, 96, 046803.
30. Bus, E.; Miller, J. T.; van Bokhoven, J. A. Hydrogen
Chemi-sorption onAl2O3-Supported Gold Catalysts. J. Phys. Chem.B
2005, 109, 14581–14587.
31. Driessen, A.; Sanger, P.; Hemmes, H.; Griessen, R.
MetalHydride Formation at Pressures up to 1 Mbar. J. Phys.:Condens.
Matter 1990, 2, 9797.
32. McLellan, R. Solid Solutions of Hydrogen inGold, Silver
andCopper. J. Phys. Chem. Solids 1973, 34, 1137–1141.
33. Schmidbaur, H.; Raubenheimer, H. G.; Dobrza�nska, L.
TheGold�Hydrogen Bond, Au�H, and the Hydrogen Bond toGold, AuH�X.
Chem. Soc. Rev. 2014, 43, 345–380.
34. Giangregorio, M. M.; Losurdo, M.; Bianco, G. V.;
Operamolla,A.; Dilonardo, E.; Sacchetti, A.; Capezzuto, P.;
Babudri, F.;Bruno, G. Insight into Gold Nanoparticle�Hydrogen
Inter-action: A Way to Tailor Nanoparticle Surface Charge
andSelf-Assembled Monolayer Chemisorption. J. Phys. Chem. C2011,
35. Kang, G.-J.; Chen, Z.-X.; Li, Z.; He, X. A Theoretical Study
ofthe Effects of the Charge State and Size of Gold Clusters onthe
Adsorption andDissociation of H2. J. Chem. Phys. 2009,130,
36. Bus, E.; van Bokhoven, J. A. Hydrogen Chemisorption
onSupported Platinum, Gold, and Platinum�Gold-Alloy Cat-alysts.
Phys. Chem. Chem. Phys. 2007, 9, 2894–2902.
37. Boronat, M.; Concepción, P.; Corma, A.; González, S.; Illas,
F.;Serna, P. A Molecular Mechanism for the
ChemoselectiveHydrogenation of Substituted Nitroaromatics with
Nano-particles of Gold on TiO2 Catalysts: A Cooperative
Effectbetween Gold and the Support. J. Am. Chem. Soc. 2007,129,
38. Schwerdtfeger, P.; Boyd, P. D. W.; Brienne, S.; Burrell, A.
K.Relativistic Effects in Gold Chemistry. 4. Gold(III) and Gold-(V)
Compounds. Inorg. Chem. 1992, 31, 3411–3422.
39. Govorov, A. O.; Zhang, H.; Gunko, Y. K. Theory of
Photo-injection of Hot Plasmonic Carriers from Metal
Nanostruc-tures into Semiconductors and Surface Molecules. J.
Phys.Chem. C 2013, 117, 16616–16631.
40. Janssens, T. V. W.; Clausen, B. S.; Hvolbaek, B.; Falsig,
H.;Christensen, C. H.; Bligaard, T.; Norskov, J. K. Insights
intothe Reactivity of Supported Au Nanoparticles: CombiningTheory
and Experiments. Top. Catal. 2007, 44, 15–26.
41. Lyalin, A.; Taketsugu, T. A Computational Investigation ofH2
Adsorption and Dissociation on Au NanoparticlesSupported on TiO2
Surface. Faraday Discuss. 2011, 152,185–201.
42. Haiss, W.; Thanh, N. T.; Aveyard, J.; Fernig, D. G.
Determina-tion of Size and Concentration of Gold Nanoparticles
fromUV-Vis Spectra. Anal. Chem. 2007, 79, 4215–4221.
43. Sanz, J. M.; Ortiz, D.; Alcaraz de la Osa, R.; Saiz, J.
M.;González, F.; Brown, A. S.; Losurdo, M.; Everitt, H.; Moreno,F.
UV Plasmonic Behavior of Various Metal Nanoparticles
SIL ET AL . VOL. 8 ’ NO. 8 ’ 7755–7762 ’ 2014
in the Near-and Far-Field Regimes: Geometry and Sub-strate
Effects. J. Phys. Chem. C 2013, 117, 19606–19615.
44. Albella, P.; Garcia-Cueto, B.; González, F.; Moreno, F.;
Wu,P. C.; Kim, T.-H.; Brown, A.; Yang, Y.; Everitt, H. O.; Videen,
G.Shape Matters: Plasmonic Nanoparticle Shape EnhancesInteraction
with Dielectric Substrate. Nano Lett. 2011, 11,3531–3537.
45. Jain, P. K.; Lee, K. S.; El-Sayed, I. H.; El-Sayed, M. A.
Calcu-lated Absorption and Scattering Properties of
GoldNanoparticles of Different Size, Shape, and
Composition:Applications in Biological Imaging and Biomedicine. J.
Phys.Chem. B 2006, 110, 7238–7248.
46. Grammatikopoulos, S.; Pappas, S. D.; Dracopoulos,
V.;Poulopoulos, P.; Fumagalli, P.; Velgakis, M. J.; Politis,
C.Self-Assembled Au Nanoparticles on Heated CorningGlass by Dc
Magnetron Sputtering: Size-Dependent Sur-face Plasmon Resonance
Tuning. J. Nanopart. Res. 2013,15, 1–8.
47. Stobi�nski, L.; Nowakowski, R.; Du�s, R. Atomic
HydrogenAdsorption on Thin Discontinuous and Continuous
GoldFilms;Similarities and Differences. Vacuum 1997,
48. Aruda, K. O.; Tagliazucchi, M.; Sweeney, C. M.; Hannah,D.
C.; Schatz, G. C.; Weiss, E. A. Identification of Parametersthrough
Which Surface Chemistry Determines the Life-times of Hot Electrons
in Small Au Nanoparticles. Proc.Natl. Acad. Sci. U.S.A 2013, 110,
49. Link, S.; El-Sayed, M. A. Spectral Properties and
RelaxationDynamics of Surface Plasmon Electronic Oscillations
inGold and Silver Nanodots and Nanorods. J. Phys. Chem. B1999, 103,
50. Libisch, F.; Cheng, J.; Carter, E. A.
Electron-Transfer-InducedDissociation of H2 on Gold Nanoparticles:
Excited-StatePotential Energy Surfaces via Embedded
CorrelatedWavefunction Theory. Masthead 2013, 227.
51. Schmickler, W.; Santos, E. Interfacial
Electrochemistry;Oxford University Press: New York, 1996; Vol. 134,
52. Thompson, C. V. Solid-State Dewetting of Thin Films.
Annu.Rev. Mater. Res. 2012, 42, 399–434.
53. Necas, D.; Klapetek, P. Gwyddion: An Open-Source Soft-ware
for SPM Data Analysis. Cent. Eur. J. Phys. 2012, 10,181–188.
54. Draine, B. T.; Flatau, P. J. Discrete-Dipole Approximation
forScattering Calculations. JOSA A 1994, 11, 1491–1499.
55. Palik, E. D. Handbook of Optical Constants of
Solids;Academic Press: New York, 1998; Vol. 3.
56. Plimpton, S. Fast Parallel Algorithms for
Short-RangeMolecular Dynamics. J. Comput. Phys. 1995, 117,